#------------------------------------------------------------------------------
#$Date: 2019-11-23 05:35:19 +0200 (Sat, 23 Nov 2019) $
#$Revision: 232238 $
#$URL: file:///home/coder/svn-repositories/cod/cif/4/34/72/4347266.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4347266
loop_
_publ_author_name
'Li, Li'
'Nishihara, Sadafumi'
'Inoue, Katsuya'
'Kurmoo, Mohamedally'
_publ_section_title
;
 Progressive Transformation between Two Magnetic Ground States for One
 Crystal Structure of a Chiral Molecular Magnet.
;
_journal_issue                   6
_journal_name_full               'Inorganic chemistry'
_journal_page_first              3047
_journal_page_last               3057
_journal_paper_doi               10.1021/acs.inorgchem.5b02956
_journal_volume                  55
_journal_year                    2016
_chemical_formula_sum            'C5 H9 Mn1.33 N4 O3'
_chemical_formula_weight         246.41
_space_group_IT_number           173
_space_group_name_Hall           'P 6c'
_space_group_name_H-M_alt        'P 63'
_symmetry_cell_setting           hexagonal
_symmetry_space_group_name_H-M   'P 63'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                120.00
_cell_formula_units_Z            6
_cell_length_a                   13.5214(11)
_cell_length_b                   13.5214(11)
_cell_length_c                   8.0686(6)
_cell_measurement_reflns_used    5913
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      27.70
_cell_measurement_theta_min      3.01
_cell_volume                     1277.53(18)
_computing_cell_refinement       'Bruker SAINT'
_computing_data_collection       'Bruker APEX2'
_computing_data_reduction        'Bruker SAINT'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.976
_diffrn_measured_fraction_theta_max 0.976
_diffrn_measurement_device_type  'Bruker APEX-II CCD'
_diffrn_measurement_method       'φ and ω scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0234
_diffrn_reflns_av_sigmaI/netI    0.0278
_diffrn_reflns_limit_h_max       14
_diffrn_reflns_limit_h_min       -17
_diffrn_reflns_limit_k_max       16
_diffrn_reflns_limit_k_min       -15
_diffrn_reflns_limit_l_max       10
_diffrn_reflns_limit_l_min       -9
_diffrn_reflns_number            9250
_diffrn_reflns_theta_full        27.85
_diffrn_reflns_theta_max         27.85
_diffrn_reflns_theta_min         3.01
_diffrn_standards_number         0
_exptl_absorpt_coefficient_mu    2.003
_exptl_absorpt_correction_T_max  0.9242
_exptl_absorpt_correction_T_min  0.6901
_exptl_absorpt_correction_type   multi-scan
_exptl_crystal_colour            black
_exptl_crystal_density_diffrn    1.922
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       prism
_exptl_crystal_F_000             746
_exptl_crystal_size_max          0.20
_exptl_crystal_size_mid          0.04
_exptl_crystal_size_min          0.04
_refine_diff_density_max         0.550
_refine_diff_density_min         -0.338
_refine_diff_density_rms         0.071
_refine_ls_abs_structure_details 'Flack H D (1983), Acta Cryst. A39, 876-881'
_refine_ls_abs_structure_Flack   0.04(2)
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.087
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     121
_refine_ls_number_reflns         1874
_refine_ls_number_restraints     1
_refine_ls_restrained_S_all      1.087
_refine_ls_R_factor_all          0.0329
_refine_ls_R_factor_gt           0.0266
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0277P)²+0.3916P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0552
_refine_ls_wR_factor_ref         0.0569
_reflns_number_gt                1725
_reflns_number_total             1874
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ic5b02956_si_002.cif
_cod_data_source_block           L1-FI*_293K
_cod_depositor_comments
;
The following automatic conversions were performed:

data item '_symmetry_cell_setting' value 'Hexagonal' was changed to
'hexagonal' in accordance with the
/home/saulius/struct/COD-crude-data/automatic-downloads/DataCite-retrospective/ACS/depositions/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 last updated on
2011-04-26.

Automatic conversion script
Id: cif_fix_values 6909 2019-04-08 15:41:33Z antanas 
;
_cod_original_sg_symbol_H-M      P6(3)
_cod_database_code               4347266
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, z+1/2'
'-y, x-y, z'
'-x+y, -x, z'
'x-y, x, z+1/2'
'y, -x+y, z+1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
Mn2 Mn 0.3333 0.6667 0.92189(8) 0.01463(14) Uani 1 3 d S
Mn1 Mn 0.30139(3) 0.33802(3) 0.54531(5) 0.02261(11) Uani 1 1 d .
O2 O 0.23003(17) 0.18142(15) 0.4068(3) 0.0348(5) Uani 1 1 d .
C5 C 0.53482(19) 0.32273(18) 0.5486(4) 0.0210(5) Uani 1 1 d .
C4 C 0.3537(2) 0.5599(2) 0.7766(3) 0.0213(6) Uani 1 1 d .
O1 O 0.24578(17) 0.05806(16) 0.2468(2) 0.0308(5) Uani 1 1 d .
C1 C 0.2677(2) 0.1579(2) 0.2803(3) 0.0237(6) Uani 1 1 d .
N1 N 0.3468(2) 0.2087(2) 0.0007(3) 0.0308(6) Uani 1 1 d .
H1A H 0.4112 0.2567 -0.0541 0.037 Uiso 1 1 calc R
H1B H 0.2865 0.1987 -0.0596 0.037 Uiso 1 1 calc R
C2 C 0.3456(2) 0.2547(2) 0.1639(3) 0.0213(5) Uani 1 1 d .
H1 H 0.4231 0.2872 0.2084 0.026 Uiso 1 1 calc R
N2 N 0.3658(2) 0.42760(19) 0.3033(3) 0.0285(5) Uani 1 1 d .
H2A H 0.3482 0.4834 0.2956 0.034 Uiso 1 1 calc R
H2B H 0.4425 0.4608 0.3020 0.034 Uiso 1 1 calc R
C3 C 0.3195(3) 0.3525(2) 0.1567(4) 0.0316(7) Uani 1 1 d .
H2 H 0.3527 0.3970 0.0570 0.038 Uiso 1 1 calc R
H3 H 0.2375 0.3213 0.1517 0.038 Uiso 1 1 calc R
N4 N 0.4560(2) 0.3214(2) 0.6037(3) 0.0308(6) Uani 1 1 d .
N3 N 0.3680(2) 0.5000(2) 0.6910(3) 0.0342(6) Uani 1 1 d .
O3 O 0.3333 0.6667 0.4001(11) 0.157(3) Uani 1 3 d S
O5 O 0.0000 0.0000 0.089(5) 0.333(10) Uani 1 3 d S
O4 O 0.0000 0.0000 0.3669(4) 0.0184(7) Uani 1 3 d S
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mn Mn 0.3368 0.7283 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
C4 Mn2 C4 88.61(11) . 4_565
C4 Mn2 C4 88.61(11) . 3_665
C4 Mn2 C4 88.61(11) 4_565 3_665
C4 Mn2 C5 173.43(12) . 6_565
C4 Mn2 C5 90.20(10) 4_565 6_565
C4 Mn2 C5 84.91(10) 3_665 6_565
C4 Mn2 C5 90.20(11) . 5
C4 Mn2 C5 84.91(10) 4_565 5
C4 Mn2 C5 173.43(12) 3_665 5
C5 Mn2 C5 96.13(12) 6_565 5
C4 Mn2 C5 84.91(10) . 2_665
C4 Mn2 C5 173.43(12) 4_565 2_665
C4 Mn2 C5 90.20(11) 3_665 2_665
C5 Mn2 C5 96.13(12) 6_565 2_665
C5 Mn2 C5 96.13(12) 5 2_665
O2 Mn1 O1 89.04(8) . 5
O2 Mn1 N2 86.61(8) . .
O1 Mn1 N2 161.05(8) 5 .
O2 Mn1 N3 177.49(9) . .
O1 Mn1 N3 89.53(9) 5 .
N2 Mn1 N3 94.09(9) . .
O2 Mn1 N4 89.57(9) . .
O1 Mn1 N4 102.29(8) 5 .
N2 Mn1 N4 96.11(9) . .
N3 Mn1 N4 92.75(9) . .
O2 Mn1 N1 89.99(9) . 5
O1 Mn1 N1 73.88(8) 5 5
N2 Mn1 N1 87.68(8) . 5
N3 Mn1 N1 87.63(9) . 5
N4 Mn1 N1 176.15(9) . 5
C1 O2 Mn1 129.45(18) . .
N4 C5 Mn2 171.4(3) . 2_664
N3 C4 Mn2 178.3(2) . .
C1 O1 Mn1 117.67(17) . 6_554
O2 C1 O1 122.7(3) . .
O2 C1 C2 118.6(2) . .
O1 C1 C2 118.7(2) . .
C2 N1 Mn1 106.53(16) . 6_554
C2 N1 H1A 110.4 . .
Mn1 N1 H1A 110.4 6_554 .
C2 N1 H1B 110.4 . .
Mn1 N1 H1B 110.4 6_554 .
H1A N1 H1B 108.6 . .
N1 C2 C1 109.8(2) . .
N1 C2 C3 113.0(2) . .
C1 C2 C3 114.0(2) . .
N1 C2 H1 106.5 . .
C1 C2 H1 106.5 . .
C3 C2 H1 106.5 . .
C3 N2 Mn1 114.26(17) . .
C3 N2 H2A 108.7 . .
Mn1 N2 H2A 108.7 . .
C3 N2 H2B 108.7 . .
Mn1 N2 H2B 108.7 . .
H2A N2 H2B 107.6 . .
N2 C3 C2 111.1(2) . .
N2 C3 H2 109.4 . .
C2 C3 H2 109.4 . .
N2 C3 H3 109.4 . .
C2 C3 H3 109.4 . .
H2 C3 H3 108.0 . .
C5 N4 Mn1 144.7(2) . .
C4 N3 Mn1 151.0(2) . .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Mn2 C4 1.983(3) .
Mn2 C4 1.983(3) 4_565
Mn2 C4 1.983(3) 3_665
Mn2 C5 1.997(3) 6_565
Mn2 C5 1.997(3) 5
Mn2 C5 1.997(3) 2_665
Mn1 O2 2.1496(19) .
Mn1 O1 2.1551(19) 5
Mn1 N2 2.232(2) .
Mn1 N3 2.240(2) .
Mn1 N4 2.261(2) .
Mn1 N1 2.298(2) 5
O2 C1 1.251(3) .
C5 N4 1.147(3) .
C5 Mn2 1.997(3) 2_664
C4 N3 1.151(4) .
O1 C1 1.258(3) .
O1 Mn1 2.1551(19) 6_554
C1 C2 1.525(4) .
N1 C2 1.460(4) .
N1 Mn1 2.298(2) 6_554
N1 H1A 0.9000 .
N1 H1B 0.9000 .
C2 C3 1.531(4) .
C2 H1 0.9800 .
N2 C3 1.479(4) .
N2 H2A 0.9000 .
N2 H2B 0.9000 .
C3 H2 0.9700 .
C3 H3 0.9700 .
O5 O4 1.79(4) 2_554
O4 O5 1.79(4) 2
loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
O1 Mn1 O2 C1 -164.1(3) 5
N2 Mn1 O2 C1 34.3(3) .
N3 Mn1 O2 C1 141(2) .
N4 Mn1 O2 C1 -61.8(3) .
N1 Mn1 O2 C1 122.0(3) 5
C4 Mn2 C4 N3 113(8) 4_565
C4 Mn2 C4 N3 25(8) 3_665
C5 Mn2 C4 N3 34(9) 6_565
C5 Mn2 C4 N3 -162(8) 5
C5 Mn2 C4 N3 -66(8) 2_665
Mn1 O2 C1 O1 152.1(2) .
Mn1 O2 C1 C2 -26.5(4) .
Mn1 O1 C1 O2 -170.8(2) 6_554
Mn1 O1 C1 C2 7.8(3) 6_554
Mn1 N1 C2 C1 -36.4(2) 6_554
Mn1 N1 C2 C3 -164.88(19) 6_554
O2 C1 C2 N1 -159.7(2) .
O1 C1 C2 N1 21.6(3) .
O2 C1 C2 C3 -31.8(4) .
O1 C1 C2 C3 149.6(3) .
O2 Mn1 N2 C3 10.37(18) .
O1 Mn1 N2 C3 -66.7(3) 5
N3 Mn1 N2 C3 -167.22(19) .
N4 Mn1 N2 C3 99.56(19) .
N1 Mn1 N2 C3 -79.76(19) 5
Mn1 N2 C3 C2 -57.7(3) .
N1 C2 C3 N2 -155.6(2) .
C1 C2 C3 N2 78.1(3) .
Mn2 C5 N4 Mn1 9.6(17) 2_664
O2 Mn1 N4 C5 67.2(4) .
O1 Mn1 N4 C5 156.1(3) 5
N2 Mn1 N4 C5 -19.4(4) .
N3 Mn1 N4 C5 -113.8(4) .
N1 Mn1 N4 C5 150.5(12) 5
Mn2 C4 N3 Mn1 -160(8) .
O2 Mn1 N3 C4 13(3) .
O1 Mn1 N3 C4 -41.9(5) 5
N2 Mn1 N3 C4 119.5(5) .
N4 Mn1 N3 C4 -144.1(5) .
N1 Mn1 N3 C4 32.0(5) 5
